Retention of Implant Supported Metal Crowns Cemented with Different Luting Agents: A Comparative Invitro Study
Roohi Kapoor1, Kavipal Singh2, Simrat Kaur3, Aman Arora4
ABSTRACT Introduction: To overcome limitations of screw-retained prostheses, cement-retained prostheses have become the restoration of choice now a days. Selection of the cement hence becomes very critical to maintain retrievability of the prostheses. Aim: The purpose of this study was to assess and compare the retention of base metal crowns cemented to implant abutments with five different luting cements. Materials and Methods: Ten implant analogs were secured in five epoxy resin casts perpendicular to the plane of cast in right first molar and left first molar region and implant abutments were screwed. Total of 100 metal copings were fabricated and cemented. The cements used were zinc phosphate, resin modified glass ionomer cement, resin cement, non-eugenol acrylic based temporary implant cement & non-eugenol temporary resin cement implant cement. Samples were subjected to a pull-out test using an Instron universal testing machine at a crosshead speed of
0.5mm/min. The load required to de-cement each coping was recorded and mean values for each group calculated and put to statistical analysis. Results: The results showed that resin cement has the highest retention value 581.075N followed by zinc phosphate luting cement 529.48N, resin modified glass ionomer cement 338.095 N, non-eugenol acrylic based temporary implant cement 249.045 N and non-eugenol temporary resin implant cement 140.49N. Conclusion: Within the limitations of study, it was concluded that non-eugenol acrylic based temporary implant cement and non-eugenol temporary resin implant cement allow for easy retrievability of the prosthesis in case of any failure in future. These are suitable for cement retained implant restorations. The results provide a possible preliminary ranking of luting agents based on their ability to retain an implant-supported prosthesis and facilitate easy retrieval.
Keywords: Implant restorations, Luting cement, Retrievability, Retention test
INTRODUCTION Implant supported restorations can be attached to implants with screws or can be cemented to abutments which are secured to implants with screws. Screw-retained prostheses have a welldocumented history of successful application in completely edentulous patients . In the areas of limited interridge space, a screw is more effective because abutment lacks the factors of height and surface area. Screw–retained, implant-supported crowns produce tighter margins . However, due to the absence of passive fit of screw-retained superstructures there is greater stress concentration around the implants . To overcome the limitations of screw-retained prostheses, cementretained prosthesis have become the restoration of choice for the treatment of implant patients. Cemented prosthesis has superior occlusion, aesthetics and loading characteristics when compared with screw-retained prosthesis . The main disadvantage of cemented prosthesis is their irretrievability . Implant screw joints are susceptible to screw loosening or fracture because of the magnitude and direction of oral forces and the strength limitations of the components. Screw- related complications may be difficult to manage especially when prosthesis has been permanently cemented . On the other hand, the selection of cement that is not retentive enough could be a possible source of embarrassment for the patient .
2014). The retention test were performed in CIPET (Central Institute of Plastic Engineering and Technology), Amritsar, India. In the present invitro study, five epoxy resin edentulous maxillary casts were fabricated. An acrylic resin model of edentulous maxilla was used to form a mold for fabricating epoxy resin cast. Epoxy resin (Araldite CY 230-1 IN, India) was mixed with the hardner (Hunstsman advanced materials LLC, USA, Aradur HY 951, India) in ratio of 10:1 as recommended by the manufacturer. The mixture was poured into the mold and allowed to set at room temperature. After 24 hours, the epoxy resin cast was obtained, finished and polished. The holes for implant analogs were milled in all the five epoxy resin casts, perpendicular to the plane of cast in right first molar and left first molar region with help of milling machine (CNC Milling machine, model no. UME-600, Mikron) [Table/Fig-2] and implant analogs (Internal hex, Adin dental implant systems ltd, Israel) were secured with help of clear autopolymerizing acrylic resin (Rapid Repair, Pyrex, India) [Table/Fig-3]. The implant abutments (Adin dental implant systems Ltd, Israel, 4mm in diameter and 11mm height) were screwed into all the analogs with help of hex driver (Adin dental implant systems ltd, Israel) [Table/Fig-4] and torqued to 30N cm S.No
Groups (Sample Size)
Group I (N-20)
Zinc Phosphate (Harvard)
The study aimed to assess and compare the retention of base metal crowns cemented to implant abutments with five cements i.e. zinc phosphate, resin modified glass ionomer cement, resin cement, non-eugenol acrylic based temporary implant cement & non-eugenol temporary resin cement [Table/Fig-1].
Group II (N-20)
Resin Modified Glass Ionomer (Rely X Luting 2)
Group III (N-20)
Resin Cement (Rely X U200)
Group IV (N-20)
Non-Eugenol Acrylic Based Temporary Cement (Improv)
MATERIALs AND METHODS
Group V (N-20)
The study was conducted in Sri Guru Ram Das Institute of Dental Sciences & Research, Amritsar for a period of one year (2013-
Non-Eugenol Temporary Resin Cement (Premier)
[Table/Fig-1]: Showing various cements used.
Journal of Clinical and Diagnostic Research. 2016 Apr, Vol-10(4): ZC61-ZC64
Roohi Kapoor et al., Retention of Implant Metal Crowns Cemented with Five Luting Agents
with torque wrench. Total of 20 metal crowns (ten on left implant analog and ten on the right implant analog in the first molar region) were fabricated on each epoxy resin cast and total being 100. The access holes in the abutments were filled with cotton plug and sealed with clear autopolymerising acrylic resin (Rapid Repair, Pyrex, India). One layer of die spacer (Gold, 15µm, Duralon) was applied on the abutment 1mm short of the margin with help of brush and was allowed to dry. After that, one layer of die lubricant was applied with help of brush and allowed to dry. Wax pattern of a crown was made with inlay wax (Bego, Germany). An 8mm diameter loop of wax was added to the occlusal surface of each crown for retention test. The wax patterns were invested in a phosphate-bonded investment (Bellavest®, Bego, Germany) and casting was done in non-precious metal alloy (Wiron® 99, Bego, Germany) in the induction casting machine (Bego, Germany). The castings were evaluated and adjusted, if any and the metal crowns were finished, polished and cemented [Table/Fig-5]. Cemented crowns were pulled off with a crosshead speed of 1mm/ min, and the maximum force to debond each crown was considered as retentive strength [Table/Fig-6] as mentioned in [Table/Fig-7]. Data thus obtained was put to statistical analysis (One-way ANOVA and Post-hoc Tukey test) and graph was plotted [Table/Fig-8].
[Table/Fig-2]: Milling of epoxy resin casts.
In group I mean retentive strength was 529.480±35.861 with range of 460.0 – 594.6. In group II mean retentive strength was 338.095±31.098 with range of 274.5 – 381.7. In group III mean retentive strength was 581.075±21.552 with range of 539.4 – 627.1. In group IV mean retentive strength was 249.045 ± 14.876 with range of 224.80 – 276.06. In group V mean retentive strength was 140.490 ± 4.832 with range of 133.4 – 150.5 [Table/Fig-7]. Comparing mean retentive strength among five groups using one-way ANOVA, F value came out to be 1166.993 and p-value was